Mechanical and Durability Performance of High-Strength Concrete with Waste Tyre Steel Fibres

Pan-African University, Institute for Basic Sciences, Technology and Innovation Hosted at Jomo Kenyatta University of Agriculture and Technology (JKUAT), Nairobi, Kenya Department of Building and Civil Engineering, Technical University of Mombasa (TUM), Mombasa, Kenya Department of Civil, Construction and Environmental Engineering, Jomo Kenyatta University of Agriculture and Technology (JKUAT), Nairobi, Kenya Department of Agricultural and Biosystems Engineering, Jomo Kenyatta University of Agriculture and Technology (JKUAT), Nairobi, Kenya


Introduction
Fibre-reinforced concrete has been used in the building industry over the years, particularly when structural engineers require the initial improvement of the mechanical properties of concrete. In most developing countries, there is a high rate of waste tyres due to the importation of used cars. e waste tyres increase the burden on the environment because they are resistant to degradation in land lls. According to National Transport Service Authority in Kenya, 90,000 vehicles were registered in 2019 with a forecast of 1.35 million vehicles in 2030. ese cars produce several sets of waste tyres during a lifetime, increasing the demand for their reuse. To develop an effective alternative for the disposal of waste tyres in East African cities while improving the properties of concrete composites, the reuse of steel fibres from the pyrolysis process of used car tyres is the paramount aspect to investigate. Past studies have investigated the importance of reusing rubber in cementitious composites such as blocks and concrete as recyclability practices of the waste tyre [1,2]. However, in these studies and in many pyrolysis processes, less emphasis is placed on how to protect the environment against residual steel fibres. Fibre-reinforced concrete is required in infrastructures where electromagnetic neutrality is required and where lightweight structures are required [3]. Along with the use of fibres in concrete, the sustainable use of natural resources needs an emphasis. e application of aggregates in the construction industry can be minimized by reducing the size of structural elements. is is achieved by adopting highstrength concrete. An increase in the concrete grade of more than 50 MPa results in a concrete with less ductility, which is prone to failure in tensile load configurations. e ductility in the structure can significantly resist the devastating failure under seismic load, provide a warning before the failure of the structures, and delay the formation of rapid plasticity in structural elements such as beams [4,5]. e ductility of high-strength concrete can be improved by incorporating fibres into the matrix. Concrete with high fibre content has a high dynamic increase factor and general dynamic responses, resulting in high resistance to structural failure under dynamic excitation [6]. Several studies agree that the inclusion of straight fibres in concrete improves its tensile and flexural strength under monolithic loading. However, this has less influence on shear resistance and compressive strength of concrete with fibre content more than 1.0% [7,8]. e reduction in compressive strength is associated with the excessive congestion of the fibres in the matrix, leading to less binder across the fibres resulting in weak zones and low bonds in the matrix [9]. Compressive strength is a key aspect of shear transfer in a concrete section. erefore, a low compressive resistance could lead to a weak fibre-concrete interface that could affect the shear transfer mechanism of the fibre. Fibre in concrete matrix under shear transfers shear in terms of compressive strain [10]. Despite the shear transfer by fibre, the inclusion of fibres improves the load-carrying capacity after first crack (strain hardening). e study by [11] concluded that fibre content between 0 and 3% increases the flexural strength by 244%. is increase advances the postbehaviour of fibrereinforced concrete to carry more loads.
To facilitate load transfer in concrete, the shape and surface texture of the fibres play an important role. For instance, the hooked-end fibres offer high resistance to concrete pullout under tension. Previous studies [12,13] hypothesized that hook fibres have high contact pressure in the localized area of the hook compared to straight steel fibres. is pressure leads to high friction stresses when the matrix is loaded that contribute to the bond strength of the matrix at the initial damage/cracking of fibre-concrete interface. Despite that hooked steel fibres are the best for improving mechanical properties up to 1.5% fibre content, most of these are synthetic/industrial fibres that are economically unviable in the construction industry compared to straight waste tyre steel fibres. According to [14], concrete with a 1% content of industrial fibres increases the cost of production and increases carbon emissions to about 84.4% and 58%, respectively.
High-strength concrete has a dense matrix that improves its performance in terms of durability compared to normal concrete [15,16]. However, the inclusion of fibres can trigger this performance in the area with high humidity and high concentration of chloride ions. Due to the variability of steel fibres in tyres, the extent of their performance in concrete has not been well established. To date, research on the mechanical properties of concrete has mostly focused on the utilization of industrial steel fibres. However, the field of durability and mechanical performance of composites with waste tyre steel fibres is drawing growing attention due to the environmental demand for these wastes and the required ductility of HSC. erefore, this work aims to broaden the understanding of the effects of waste tyre fibres on Poisson's ratio, the ingress of harmful chemicals, sorptivity, and the mechanical properties of high-strength concrete (HSC).

Materials.
Bamburi Portland cement CEM I 42.5 was used in this study as per EN197-1 [17]. e coarse and fine aggregates were sourced from Mlolongo quarries in Nairobi, Kenya.
e coarse aggregates had a maximum size of 12.5 mm. To maintain the flowability of the concrete matrix, Sika Viscocrete 3088 superplasticiser was also used. is superplasticiser type is a high-range water-reducing admixture (HRWRA). It has a density of 1.05 kg/litre and a pH of 4.5 ± 0.5 according to the manufacturer product data sheet. e steel fibres that were used in this study were processed by pyrolysis in a plant in the Athi River area, Machakos County, Kenya. A summary of the materials used in the study is presented in Table 1.

Characterization of Aggregates.
e coarse aggregates were sieved and graded according to ASTM 33 [18]. Relative densities of aggregates were determined as per BS 812 [19]. e determination of relative densities for fine and coarse aggregates involved some steps, such as weighing the mass of the pycnometer with sand-and air-drying of coarse aggregates, as shown in Figures 1(a) and 1(b), respectively. e fineness modulus of the coarse and fine aggregates was 2.5 and 2.4, falling within the acceptable range of 2.4 to 3.1 for the aggregates to be accepted for concrete production. e grading curves of the aggregates are shown in Figure 2.

Physical and Mechanical Properties of Aggregates.
e results of the physical and mechanical properties of the aggregates used in this study are shown in Table 2. Coarse aggregates and fine aggregates with dry-bulk density rolls of 1642 kg/m 3 and 1516 kg/m 3 were used. e coarse aggregates had an aggregate impact value (AIV) and an aggregate 2 Advances in Civil Engineering crushing value (ACV) of 6.2% and 18.2%, less than 10% and 30%, respectively, according to the CML [20].

Characterization of Waste Tyre
Fibres. e waste tyre steel fibres were cut into lengths measuring 30, 50, and 60 mm using a bolt clipper. An effective fibre length of 200 mm was used to determine the tensile strength and elongation of the steel fibres using the Hounsfield tensometer as shown in Figure 3(a). Due to the contamination of oil and black carbon in the burning process of tyres, the fibres were washed and dried before they were added to concrete.

Physical and Mechanical Properties of Waste Tyre Steel
Fibres.
e fibre characterization was performed, and the properties are shown in Table 3. e fibre cord had twentyseven tiny fibres in it. e fibre had a tensile force and elongation of 901 N and 8 mm, respectively. e average tensile strength of the fibres is consistent with ASTM A820 [21]. Virgin tyre steel cord with a diameter greater than 1.3 mm has a tensile force greater than 1000 N [22]. e small tensile force of the fibre in this study is associated with the high temperature (750°C) used in the tyre burning process. At this temperature, there are microstructural changes in the fibre that result in new sets of defective threads, making it easy for these fibres to break [23,24].

Mixing Proportions.
e target mean compressive strength was 70 MPa. e mix proportions were prepared according to ACI 211 [25], in which the water-to-cement ratio of 0.36 was adopted. To increase workability, a superplasticiser dosage of 0.9% of the weight of cement was used in each mix proportion as more dosage of 1.2% can compromise the properties of concrete [26,27]. For each length of fibres, the study adopted four different contents as percentages of the density of steel (i.e., 7850 kg/m 3 based on literature). e percentages of fibres with respect to their weight in a cubic metre of concrete and the proportions of the mix are given in Tables 4 and 5, respectively.

Compressive Strength Test and Workability.
After classification of the materials, concrete cubes measuring 100 × 100 × 100 mm were cast and cured in water for 3, 7, and 28 days for the control mix and 12 sets of specimens with fibres. In each period of curing, three cubes were tested. e workability of concrete in each mix was assessed using a slump cone of 300 mm high in which a slump ruler was used to quantify the slump value as shown in Figure 4. e compressive test was carried out using a universal tensile machine with a capacity of 1500 kN at a load rate of 0.5 kN/s according to EN 12390-3 [28]. e average of three cubes determined the crushing strength of the concrete. Before testing for each period, the concrete cubes were air-dried for one hour to dry the surfaces.

Splitting Tensile Strength Test.
To determine the splitting tensile strength, thirteen sets of specimens, namely, control mix, and twelve sets with fibres were considered. ree concrete cylinders were cast and tested for each set on the 28 curing days. e cylinder mould used had diameter of 100 mm and a height of 200 mm. Splitting tensile strength of concrete was performed using the universal tensile machine (UTM), according to EN 12390-6 [29]. e concrete cylinder was placed in the UTM centred between loading plates with a loading rate of 0.1 kN/s until the failure of the specimen.

Flexural Strength Test.
e test was carried out using thirteen sets of specimens, namely, control mix and twelve sets with fibres. In each set, three concrete beams with dimensions 150 × 150 × 500 mm were cast and tested for 28 days to determine the flexural strength of high-strength concrete.
e test setup was in accordance with ASTM C1018 [30], in which a four-point load system was adopted. A hydraulic jack and load cell of capacities 40 tons and 500 kN, respectively, were used to determine the maximum flexural load. To monitor the deflection, a 20 mm dial gauge was mounted as shown in Figure 5. Load cell and dial gauge were all connected to a data logger in which calibration of load cell and dial gauge was performed before applying jack loads. An average of the three beams determined the flexural strength. Also, the flexural toughness and residual strength at l/150 were evaluated as described in ASTM C1609 [31].

Static Modulus and Poisson's Ratio.
In order to determine the static modulus and Poisson's ratio, thirteen sets of specimens, namely, control mix and twelve sets with fibres were considered. ree concrete cylinders were cast and tested for each set on 28 curing days. A 100 mm diameter and 200 mm high cylinder mould was used in the test setup. Two bonded strain gauges, each placed parallel to the axis (both vertical and horizontal axis) and circumferentially mounted at diametrically opposite gauge lines at the midheight of the concrete cylinder as shown in Figure 6, were used. Each concrete cylinder was set in compression, and these four strain gauges were connected to a data logger. Both the modulus of elasticity and Poisson's ratio were computed based on the working stress of 40% of the ultimate crushing strength of the concrete cylinder as per ASTM C469 [32].

Durability Tests
(1) Sorptivity. e test was carried out using thirteen sets of specimens, namely, control mix and twelve sets with fibres.
In each set, three cubes measuring 100 × 100 × 100 mm were tested at 28 curing days to assess the absorption rate. Before the test setup, three cubes in each set were baked in the oven for 24 hours. e oven-dried and cooled samples were covered with a plastic sheet on the top and sealed on all sides. ese samples were placed in the container with water to allow only the bottom side of the concrete to be in contact with water. e samples were removed from the container and weighed, and the values were recorded at intervals as described in ASTM C1585 [33].  (2) Chloride Ion Penetration. Twelve sets of concrete with fibres and control mix were used to assess the depth of chloride ions. In each set, three concrete cylinders measuring 100 mm diameter and 200 mm high were cast and cured for 28 days. e samples were then cured in sodium chloride (NaCl) solution for another 28 and 56 days. e curing solution of NaCl contained 3 g of NaCl in 100 ml of water. After curing in NaCl solution, 0.1 M silver nitrate (AgNO 3 ) equivalent to 1.691 g in 100 ml of water was prepared and spread on the separated faces of the concrete cylinder according to ASTM C1543 [34]. e depth of penetration of chloride ions was measured when the colour changed to a white precipitate of silver chloride because of the presence of free chlorides that react with silver nitrate and brown precipitates of silver oxide in the section with no chloride ions. e white colour was recorded as the depth of penetration of chloride ions at an average of 10-20 mm intervals along the length of the cylinder. e preparation of the solution and the split of the cylinders with a change in colour are shown in Figure 7. Figure 8 shows the plot of slump versus various fibre contents with the respective fibre lengths. e control mix had a slump of 90 mm after adding the superplasticiser. e slump value decreases as the content and length of fibres increase. Concrete with the labels SFRC60-0.5, SFRC50-0.5, and SFRC30-0.5 had slump values of 60, 63, and 70 mm and were 33%, 30%, and 22%, Steel fibre cord V-wire split chuck     respectively. is study confirms previous studies by [35,36] that the workability performance of high-strength concrete is affected by increasing the volume of fibre in it. Increased length and content increase the blockage of concrete ingredients and lead to an increase in the surface area of the mix. is surface area increases the requirements for admixtures and water for both workability and hydration, respectively.

Compressive Strength.
e results of compressive strength against curing age and fibre content are plotted in Figure 9. e results of this study are consistent with earlier literature studies. Compressive strength is affected by curing age, and it increases as curing age increases. e control mix showed less compressive strength compared to the concrete with fibres. e results showed that the compression strength increases for low fibre content due to the best attachment at the fibre-concrete interface. Concrete with medium fibre length of 50 mm and 0.5% fibre content had 15.2% increase in compressive strength than the control mix. e failure mode was brittle for the control mix, compared to the reinforced fibre-concrete cubes that failed with relatively little brittleness. Concrete with fibres has an embedment length that increases the strength of the matrix through friction between the fibre and the concrete surfaces that improves resistance Silver Nitrate findings are in line with the past study by [9]. Concrete with fibre length 50 mm with content more than 0.5% and all specimens of SFRC60 show less compressive strength. is is associated with an increase in weaker zones between the fibre-concrete interface due to the high content and length, which eventually reduces the compressive stiffness of the specimen. During the shrinkage process of concrete, high fibre content could reduce the contact pressure at the fibre-concrete interface that is responsible for the stress transfer. is reduction is associated with the less spacing of fibres in the matrix that reduces the area of concrete surrounding it, hence less imposed pressure after the matrix has shrunken [37].    Advances in Civil Engineering

Splitting Tensile Strength.
e results of the tensile strength of concrete are shown in Figure 10. e control mix showed explosive brittle and sudden failure compared to concrete with fibres. e addition of fibres prolongs failure due to the tension-stiffening action of the fibre in the concrete. In this study, the concrete cylinder with fibre showed high resistance after the first crack. e tensile strengths of SFRC60-1.0, SFRC50-0.5, and SFRC50-1.0 were 4.86 MPa, 4.82 MPa, and 4.8 MPa that were 21.5%, 20.5%, and 20% higher than the control mix, respectively. Tensile strength increases as the fibre content increases except for SFRC50-1.0, which showed a slight decrease in strength. e decrease in strength for a long length could be due to the rearrangement of the fibres during casting. e casting processes reduce the angle far less than 90°f rom the line of splitting force that significantly reduces the effectiveness of load transfer at the interface. e proper orientation of the fibres to the applied load increases the effectiveness of bridging the two halves of the cylinder before they are split [15]. It could also be attributed to the type of fibres used, in which, to some extent, the deformed fibre with the grip for the high fibre content can create microcracks during pulling out of the matrix when the sample is loaded. is increases the likelihood of weaker points along with the fibre-concrete interface, resulting in lower bond strength, and hence lower final tensile strength.
e results showed slightly less tensile strength compared to most of the industrial fibres as reported in [38]. is is due to the high temperatures used in the pyrolysis process and the wear of the fibres in the tyre resulting in some defective threads compared to virgin industrial fibres. Although vibration in concrete increases the densification of concrete, internal vibration as compared to external vibration has a negative effect on fibres realignment in the matrix [39].
is is accompanied by segregation of the fibres at a point where the poker vibrator is placed in the matrix, leaving the core part of the sample unreinforced. is effect is greater in small samples, that is, cubes and cylinders, compared to beams. e planned concrete at the core of the specimen loses the ability to withstand more loads as the specimen cracks or crushes due to the high brittleness of high-strength concrete. is resulted in a limited increase in tensile strength for all specimens and low compressive strength for SFRC50-0.75 and 1.0%.

Flexural Strength.
e crack pattern, the flexural strength, and the width of the crack of the concrete against the fibre content are plotted in Figures 11 and 12, respectively. Concrete with a fibre length of 50 mm clearly showed the resistance to crack as the content increases. e crack width of SFRC60-0.3 was 9 mm, 47.1% less than SFRC50-0.3, and as the fibre content increases, SFRC60-1.0 showed superior flexural strength values and a very small crack that occurred in line with the point of application of the load. SFRC60-1.0 showed an improvement in strength to 71.1% of the control mix. ese results agree with [35]. Large fibre length and high fibre content in concrete have a high-contact area that increases the individual bond forces of fibres in the matrix.
is resists the initiation of a plastic hinge after yielding composite in the middle third of the beam span length.

Effect of Fibre on Flexural Toughness and Residual
Strength.
e load-deflection curves, flexural toughness against fibre content, and residual strength against fibre content are plotted in Figures 13 and 14 is remaining strength in concrete indicates the effectiveness of fibre in its structural performance [40]. All these best flexural performances of fibre-reinforced concrete are brought by tension stiffening after the first cracking of the beam leading to strain hardening. Tension stiffening in fibre-reinforced concrete is due to friction stress generated between the fibre and the concrete surfaces, as the fibre tends to pull out from the matrix. is friction stress acts oppositely to the direction of tensile force, in which after the first crack it tends to restore the crack. For long and high content, this action of counteracting the tensile forces in the matrix enhances the postbehaviour of the beam.

Static Modulus and Poisson's Ratio.
Young's modulus against fibre content is plotted in Figure 15. e results of this study showed that less fibre content and length had a significant improvement in modulus compared to longer fibre length and content. Concrete with 30 mm length showed a linear increase in Young's modulus from 0.3% to 0.75% fibre content. is increment agrees with [41]. is could be associated with the tendency of the fibre to interlock the aggregates in the matrix and to limit the initiation and propagation of cracks. Concrete with fibre length 50 mm and 0.3% content showed the best improvement on modulus, 35.1% higher than the control mix. is is contrary to [42,43] that the optimal fibre content is limited to 0.5% only for 30 mm fibre length. ese results show that a further increase in fibre length and less content (SFRC50-0.3) could still have a better improvement in modulus. is is attributed to the type of fibre used in the study. It has grips around the fibre that increases the initial friction in the matrix before yielding, but these grips are likely to fail first before the core of the fibre. is early failure of grips increases the number of weaker interfacial transition zones (ITZs) for high content and large fibre lengths. is can lead to a reduction in the compression stiffness of the matrix and therefore a negative effect on Young's modulus. In addition, uneven distribution of fibres could increase the chances of premature failure of concrete matrix as the results showed that there was a sudden drop in modulus for SFRC 50-0.5, SFRC50-1.0, and SFRC 60-0.3. e results showed that, in the absence of an experimental test, the modulus of concrete with waste tyre steel fibres can still be estimated using empirical formulas in various codes of practice. e estimates in ACI308-08 are closer to the experimental results compared to Eurocode 2 for concrete with a fibre length of 30 mm. e control mix showed less modulus compared to the estimated values of the codes. is is due to the sudden crushing of the concrete cylinder that resulted in the highest record of longitudinal strain in the elastic zone, which is taken at 40% of ultimate stress. ere is also a bit of divergence of experimental results from these codes. is is due to the unreinforced concrete used in their establishments, in which the resistance to crushing is only due to the aggregates and the binder materials.
e results of Poisson's ratio with longitudinal strain and fibre content are shown in Figure 16.
e study showed Poisson's ratio of 0.143 for the control mix that falls within the range of 0.1 to 0.2 for high-performance concrete similar to [44,45]. is is because HSC without fibre has less elongation in the traverse at a working stress of 40% of the ultimate stress. When the fibres were added, the ductility of HSC increases leading to the bulging of the specimen in the traverse direction leading to high Poisson's ratios of more than 0.143. For instance, SFRC30-0.3 and SFRC50-0.5 had Poisson's ratio of 0.222 and 0.315, being 55.2% and 120.3% higher than control mix, respectively. e HSC with fibres showed many hair cracks before ultimate failure. e dominant failure mode for HSC without fibre and with less fibre content was long longitudinal cracks. In SFRC30, with more content than 0.3%, concrete resists more loads and a high elongation on the longitudinal axis, resulting in a reduction in Poisson's ratio.
is decrease in behaviour of Poisson's ratio was also reported in [46]. Concrete with fibre lengths of 50 and 60 mm did not show the best trend as with the fibre length of 30 mm, indicating the complexity of the orientation of large fibre lengths in the matrix. e SFRC50-1.0 had less axial deformation with relatively high lateral deformation resulting in highest Poisson's ratio indicating high ductility of the matrix. Unlike SFRC60, there was high resistance to both axial and lateral deformation due to the high internal lock of the particles in the matrix. is only caused fragmentations on the surface of the sample that is weaker compared to its inner part of the matrix, as shown in Figure 17.

Sorptivity.
e absorption rate versus fibre content is shown in Figure 18. In this study, a high absorption rate of water was observed for the first six hours, that is, the initial absorption rate compared to the secondary absorption rate. is is because of the rapid saturation of large pores just at the surface that gradually reduces the infiltration of water with time. Concrete with less fibre content and length, i.e., SFRC30-0.3 showed a bit higher sorptivity coefficients compared to the control mix. is could have been associated with the crowd of fibres on one side of the cube that increases capillaries as a result of close-connected ITZs with less binder. Large lengths with low content properly fill more voids than short fibres with the same content. For instance, SFRC60-0.3 has a sorptivity coefficient of 47.3% less than SFRC30-0.3 due to the long grips in the spiral form available in the selected fibre. is grip breaks the continuity of the fibre-matrix interface, blocks/fills the capillary pores, and reduces internal cracks due to shrinkage during hydration of concrete. is behaviour is consistent with previous studies [16,47]. It was also observed that an increase in fibre content resulted in an increase in sorptivity coefficient. e SFRC50-1.0 showed a high absorption rate compared to SFRC50-0.5.
is was in line with the finding in [48]. More fibres in concrete increase the porosity of concrete leading to rapid capillary rise in the matrix. Furthermore, the results showed the best decrease in the absorption rate of fibre-reinforced concrete (SFRC50-0.5) to 75% of the control mix. is resistance of fibre-reinforced concrete to absorb water increases the durability of the matrix through the inactive  Advances in Civil Engineering 13 process of water ionization by harmful acidic gaseous substances. ese gases could ionize water in concrete in the presence of oxygen into hydroxide ions that facilitate the electrochemical process and increase the potential risk of corrosion to the main rebar.

Chloride Ion
Penetration. e depth of chlorine ions is plotted in Figure 19. e depth of chloride penetration was initially lower for fibre lengths 30 mm and 50 mm at fibre content of 0.3% to 5.3% and 2.7%, respectively. At 1.0% fibre content, concrete with fibre length of 30 mm showed an increase of chloride ions to 6.7% as in previous study by [43]. With the increase in fibre length and content, the results showed a slight increase in depth of chloride penetration to 18.75% for SFRC60-1.0.
is increase in depth is in line with previous findings by [49]. is indicates that increasing the fibre content can increase the diffusion of chloride ions in concrete, not only due to the gradient between internal and external concentrations but also the capillary suction. Suction was more affected by changes in the microstructures of the matrix resulting from the fibres. e results showed that the depth of the chloride ion is less than 20 mm, which is the minimum required concrete cover in structural elements [50]. e use of waste steel fibres in high-strength concrete could have great potential. is could result in less effect of chloride ions to ionize water and initiate the corrosion of conventional steel reinforcement in a structural element.

Conclusions and Recommendations
In general, experimental results conclude that the compressive strength of concrete with fibre length of 50 mm and a content of 0.5% is 15.2% higher than control mix. Contrary to some findings in the literature, the synthetic/industrial fibres increase the compressive strength until the fibre content reaches 1.5%. e results of this study have shown the potential for the use of waste tyre steel fibres in concrete production rather than leaving them abandoned in the capitals of developing countries. e deformed spiral shape of fibre with more content can increase the chances of weaker spots along with the fibreconcrete interface. is could lead to a low bonding strength, resulting in an insignificant improvement in final tensile strength. e concrete beam without fibres (control mix) and all SFRC30 samples have an abrupt flexural failure, but when the length and content increase, the crack is lagged as SFRC50-1.0 has crack width 82.4% smaller compared to SFRC50-0.3. Inclusion of waste tyre fibres in concrete increases Young's modulus of elasticity. e optimal content of waste tyre fibre for the modulus of elasticity was 0.3% for 50 mm fibre length. ese fibres in concrete had superior residual strength of 5.68 MPa and flexural toughness of 142 Joule for beam SFRC60-1.0; however, a special mix design is required due to low workability. e results of this study underline that high-strength concrete with waste tyre steel fibres that can be used in the coastal areas due to the low rate of water absorption with 75% less than the control mix. is indicates the best performance against corrosion attack to the main rebars, although special treatment must be applied to the fibres that protrude on the surface of the concrete. Although this study showed performance in compressive strength at 0.5% of the fibre content and 50 mm fibre length, nothing has been examined for the fibre content between 0 and 0.3%, 0.3-0.5%, 0.5-0.75%, and 0.75-1.0%. In addition, the durability test was not performed for more than 56 days. In the future, research is recommended to evaluate the mechanical properties and attachment behaviour of the fibre-concrete interface at high temperatures. 14 Advances in Civil Engineering

Data Availability
e data used to support the findings of this study are included in the article.

Conflicts of Interest
e authors declare that they have no conflicts of interest.

Authors' Contributions
Daudi S. Augustino contributed to conceptualization, methodology, validation, formal analysis, investigation, resources, original draft writing, review and editing, and visualization. Richard O. Onchiri contributed to supervision and reviewing. Charles Kabubo contributed to supervision and reviewing. Christopher Kanali contributed to supervision and reviewing.